MASE 473: Determining Molecular Weight Using Solution Viscosity

Powerful Essays
1234 Words
Grammar
Plagiarism
Writing
Score
MASE 473: Determining Molecular Weight Using Solution Viscosity
Lab 2 Report for MATSE 473

Determining Molecular Weight using Solution Viscosity

Name: Mengfang Li

Group D Lab Partners: Michael Lorenzo, Peter Mcclure

01/24/2012

Introduction:

This lab was designed to demonstrate the method to measure the intrinsic viscosity of the prepared polystyrene. Intrinsic viscosity, which is measured from the flow time of a solution through a simple glass capillary, has considerable historical importance for establishing the very existence of polymer molecules. The aim of this lab is to estimate the molecular weight of a polystyrene sample by dilute viscometer. The viscosity average molecular weight is determined for polystyrene obtained from bulk process and solution process. The result molecular
The molecular weight is determined to be 147423 g/mol. However, the viscosity data for solution process product does not show a good fit on a straight line. While the first three data points (C1=0.0025 g/ml, C2=0.0017g/ml, C3=0.0013 g/ml) shows relatively linear behavior, the fourth data point (C4= 0.001 g/ml) has significantly deviated from the other points. This might be caused by the undissolved polystyrene which clogs up in the capillary tube and slows down the flow process. This explains why the flow time of the first concentration (C1=0.0025 g/ml) was significantly longer than the lower concentrations. As the 5ml of THF added for each run, the PS dissolves the best at the lowest concentrations. Due to the unexpected error, the intrinsic viscosity of PS (solution process) is determined as the reduced viscosity at lowest concentrations. The MW for polymer (solution process) is calculated to be 31254 …show more content…
This agrees with the experimental result in this lab. The bulk process yields the polymer with molecular weight about four times greater than that of solution process. The main reason causing the production of low MW polymer is that the solvent added (solution process) has made the monomer concentration much lower than the bulk process. In solution process, only soluble and low molecular weight polymers could be obtained because of chain transfer reactions with the solvents. The solvent in the solution process act as good heat conductor but also significantly lowered the monomer concentration. In contrast, bulk process enables high monomer concentration without addition of solvent. As a result, high MW polymers are easily obtained by bulk polymerization.

Conclusions/Overview:

All polymers increase the viscosity of the solvent in which they are dissolved.

The result of this experiment verifies the assumptions made at the beginning of lab. The bulk process yields the polymer with molecular weight greater than solution process mainly because of the high monomer concentrations of bulk process. The viscosity data for bulk process product shows a good linear behavior. While the viscosity data for solution process product contains errors due to undissolved PS in solution.

In order to obtain a better viscosity data, the prepared PS should ground into powder form before

You May Also Find These Documents Helpful

• Satisfactory Essays

To obtain the values for V_∅^∞ given in Table 6, they were fitted to equation 7. Note that prior measurements of density on poly(ethylene glycol) + water should perform to calculate the values of V_∅^∞ for the polymer. Table 3 has shown these empirical values for different molalities of poly(ethylene glycol). Some of the researchers 11, 18, 20 have proposed that the dependency of〖 V〗_∅ on the molality of the polymer is a linear function specified…

• 331 Words
• 2 Pages
Satisfactory Essays
• Good Essays

the polyaddition reaction, which is a special case of polycondensation, with the difference that the reaction product is exclusively the polymer. In the classical polycondensation reactions, the products are: the polycondensation polymer and a low molecular weight (MW) compound (water, alcohols, and so on). The fact that in the polyaddition reactions the product is only the polymer is of great technological importance, especially for the purity and the morphology of the resulting macromolecular…

• 666 Words
• 3 Pages
Good Essays
• Powerful Essays

Discuss this statement with reference to a polymer made from one of the above monomers.…

• 1084 Words
• 5 Pages
Powerful Essays
• Satisfactory Essays

The polymer precipitated as a white solid. It was washed with methanol, dried in desiccator and stored protected from light. The polymer was characterized by NMR and IR…

• 552 Words
• 3 Pages
Satisfactory Essays
• Satisfactory Essays

Polymer Chains

• 600 Words
• 3 Pages

2. We discussed how polymer linking and structure contribute to its properties. How would you expect the density, elasticity, and rigidity of a polymer that is branched to compare to one that is linear?…

• 600 Words
• 3 Pages
Satisfactory Essays
• Good Essays

Density Lab

• 536 Words
• 3 Pages

The same procedure was done for solids. We calculated the densities of 5g of sucrose, 2g of sodium acetate and 2g of naphthalene. The results showed…

• 536 Words
• 3 Pages
Good Essays
• Powerful Essays

Before we conduct the experiment, we must first understand what viscosity is. “Viscosity is the quantity that describes a fluid's resistance to flow”.1 It is essentially fluid friction and transforms kinetic energy of motion into heat energy, just as friction (“the force between surfaces in contact that resists their relative tangential motion”) does between two solid bodies. All fluids express some amount of viscosity. An ideal fluid has no internal friction between the molecules, meaning that it is not viscous. The reciprocal of viscosity is fluidity (“the physical property of a substance that enables it to flow.”)2 Thus, fluids that are high in viscosity tend to flow slower while fluids that are low in viscosity tend to flow faster. Different liquids have different forces: the larger the intermolecular force, the more viscous it is and vice versa.…

• 1599 Words
• 7 Pages
Powerful Essays
• Satisfactory Essays

Unknown liquid

• 264 Words
• 2 Pages

III. Procedure: 1.We massed an empty 10mL graduated cylinder to the nearest .01g. 2.Then, we filled the graduated cylinder with 4.0-5.0 mL of distilled water, 3.massed it to the nearest 0.1 ml and 4. recorded the data. Then to determine the density of the unknown liquid; we repeated the steps.…

• 264 Words
• 2 Pages
Satisfactory Essays
• Better Essays

In this experiment the plastic product was placed in a graduated cylinder with water 4 separate times per group member, totaling 16 experiments. First determined was the mass of the product by weighing on the scale, next determined was the displaced volume by subtracting the final volume from the initial volume of water in the graduated cylinder. The mass of the product was divided by the displaced volume to determine the density. Ranges of density for all 16 experiments were precise readings of 1.02%-1.07% with a group average of 1.04% - refer to Table #1.…

• 1060 Words
• 5 Pages
Better Essays
• Powerful Essays

following trial but with more of the solid, instead of 1 ml, 2 ml were used. The densities were found by…

• 1151 Words
• 5 Pages
Powerful Essays
• Satisfactory Essays

INTRODUCTION This is report analyses raw data from tensile test of polyethylene and polystyrene materials; thus drawing comparisons with published data of mechanical properties of polyethylene and polystyrene materials. Also how chemical structures affects mechanical properties of polyethylene and polystyrene. Background theory Mechanical properties of a material relate to its resistance to changes, e.g. when loaded, deformed, rise in temperature etc. This depends on the structure and…

• 591 Words
• 3 Pages
Satisfactory Essays
• Good Essays

As we can see the particles size was varied by varying the polymer ratio, and the hydrophobic moiety immobilized on the COS chain. For the COS, and its oleoyl-CGKRK derivatives, the complexes showed increase in the size by increasing the polymer ratio from 1 to 5 folds. Increasing the polymer ratio to 10 folds resulted in a decrease in the size. Meanwhile, in the case of saturated fatty acids including the palmitoyl-CGKRK, and stearoyl-CGKRK derivatives of chitosan, they exhibited different pattern as the polymer: siRNA weight ratio increases from 1 to 5 the particle size decrease, then it increased when the weight ratio of polymer: siRNA reached 10. Additionaly, we noticed that among the chitosan derivatives oleiyl derivative had the smallest particle size at all polymer ratios. It is clear that, the fatty acid chain and its degree of hydrophilicity had a strong impact on the polymer/siRNA complexes size, figure…

• 1779 Words
• 8 Pages
Good Essays
• Powerful Essays

The tensile strength of a material quantifies how much stress the material will endure before failing. This is very important in applications that rely upon a polymer 's physical strength or durability. For example, a rubber band with a higher tensile strength will hold a greater weight before snapping. The tensile test consists on the application of a tensile stress on a chosen specimen attached to a device that calculates the force applied on it and the elongation. Polymers or plastic as they are commonly known, consist of long molecular chains of carbon compounds. This type of long chain structure of the plastics or polymers give it special properties that may not be exist in metals. It’s very easy to change the shape of polymers because they are light and corrosion resistant. Additionally in the pure state all polymers are colourless and easy to produce any coloured products by the addition of dyes and pigments. Polymer`s physical, mechanical and electrical properties depends on its structure, temperature and bonds between the monomers.…

• 2341 Words
• 10 Pages
Powerful Essays
• Powerful Essays

The goal of this experiment was to determine the viscosity of given liquids. Two different methods were employed, the first measures time of flow of several methanol-water solutions, from point A to point B. The second method involves dropping a foreign object, in this case a sphere, into a cylinder of glycerol and measuring the time it takes for it to travel a specific distance down the tube. The viscosity of a 0%, 20%, 40%, 60%, 80% and 100% methanol by volume solutions was measured to be 0.89, 1.28, 1.53, 1.46, 1.11 and 0.54±0.001P, respectively. The falling sphere method was performed under two different temperatures. At 5.7°C the viscosity of glycerol was calculated to be 29.8±0.1P and at 22.7°C it was 6.3±0.1P.…

• 1827 Words
• 8 Pages
Powerful Essays
• Good Essays

Synthetic Polymers

• 3597 Words
• 15 Pages

Some molecules contain so many atoms (up to tens of thousands) that understanding their structure would seem to be an impossible task. By recognizing that many of these macromolecules exhibit recurring structural motifs, however, chemists have come to understand how these molecules are constructed and, further, how to synthesize them. These molecules, called polymers, fall into two classes: natural and synthetic. Natural polymers include many of the biomolecules that are essential to life: proteins, nucleic acids, and carbohydrates among them. Synthetic polymers—most of which were developed in just the last 60 or so years—include plastics, synthetic rubbers, and synthetic fibers. We shall study synthetic polymers in this Interchapter and natural polymers in the next one. Enormous industries have been built around synthetic polymer chemistry, which has profoundly changed the quality of life in the modern world. It is estimated that about half of all industrial research chemists are involved in some aspect of polymer chemistry. Few of us have not heard of nylon, rayon, polycarbonate, polyester, polyethylene, polystyrene, Teflon®, Formican®, and Saran, all of which are synthetic polymers. The technological impact of polymer chemistry is immense and continues to increase.…

• 3597 Words
• 15 Pages
Good Essays